Article Electro-Exfoliation of Graphite to Graphene in an Aqueous Solution of Inorganic Salt and the Stabilization of Its Sponge Structure with Poly(Furfuryl Alcohol)
Anna Ilnicka 1, Malgorzata Skorupska 1, Piotr Kamedulski 1 and Jerzy P. Lukaszewicz 1,2,* 1 Faculty of Chemistry, Nicolaus Copernicus University, Gagarina 7, 87-100 Torun, Poland 2 Centre for Modern Interdisciplinary Technologies, Nicolaus Copernicus University, Wilenska 4, 87-100 Torun, Poland * Correspondence: [email protected]; Tel.:+48-605-314-300
Received: 28 May 2019; Accepted: 29 June 2019; Published: 3 July 2019
Abstract: We demonstrate an accessible and eﬀective technique for exfoliating graphite foil and graphite powder into graphene in a water solution of inorganic salt. In our research, we report an electrochemical cathodic exfoliation in an aqueous solution of Na2SO4. After electro-exfoliation, the resulting graphene was premixed with furfuryl alcohol (FA) and an inorganic template (CaCO3 and Na2CO3). Once FA was polymerized to poly(furfuryl alcohol) (PFA), the mixture was carbonized. Carbon bridges originating in thermally-decomposed PFA joined exfoliated graphene ﬂakes and stabilized the whole sponge-type structure after the nano-template was removed. Gases evolved at the graphite electrode (cathode) played an important role in the process of graphene-ﬂake splitting and accelerated the change of graphite into graphene ﬂakes. Starting graphite materials and graphene sponges were characterized using Raman spectroscopy, SEM, high-resolution transmission electron microscopy (HRTEM), elemental analysis, and low-temperature adsorption of nitrogen to determine their structure, morphology, and chemical composition. The discovered manufacturing protocol had a positive inﬂuence on the speciﬁc surface area and porosity of the sponges. The SEM and HRTEM studies conﬁrmed a high separation degree of graphite and diﬀerent agglomeration pathways. Raman spectra were analyzed with particular focus on the intensities of ID and IG peaks; the graphene-type nature of the sponges was conﬁrmed.
Keywords: graphene; electrochemical exfoliation; aqueous solution; poly(furfuryl alcohol); Raman spectroscopy; graphite electrode
1. Introduction Graphene is a two-dimensional layer of carbon atoms which form hexagonal rings based on sp2 hybridization [1,2]. A particularly promising graphene production technique is the creation of a colloidal suspension of graphene ﬂakes or its derivatives . Unlike other methods, e.g., chemical vapor deposition, epitaxial growth, and microchemical exfoliation, this approach is versatile in terms of chemical functionalization and aﬀording the possibility of high-volume production. The latter is sometimes used to justify focus on obtaining graphene as a water dispersion . Generally, exfoliation of graphene/graphene oxide is widely exploited and was a key step in the manufacturing of complex materials like bionanocomposite based on polylactic acid , graphene oxide and biodegradable polymer blends , graphene oxide (GO) and polyamide composites, and nanosilica modiﬁed graphene . Recently, the electrochemical approach has been found to have the advantages of being single step, easy to operate, environmentally friendly, and able to operate at ambient conditions .
Nanomaterials 2019, 9, 971; doi:10.3390/nano9070971 www.mdpi.com/journal/nanomaterials Nanomaterials 2019, 9, 971 2 of 12
Graphene ﬂakes of controllable properties can be formed without the need for volatile solvents or reducing agents. The process can take several minutes or hours to complete, and the reported results are encouraging for the fast processing of large quantities of graphene ﬂakes . The electrochemical method utilizes an electrolyte solution and electrical charges to drive structural expansion and exfoliation (beside oxidation or reduction), intercalation, and exfoliation on a piece of graphite (plate, rod, wire) to produce ﬂakes. The experimental arrangement uses a monopolar, undivided electrolysis cell. The yield, productivity, and properties of graphene ﬂakes can be ﬁnetuned by controlling electrolytes and electrolysis parameters [10–12]. Electro-exfoliation has some advantages over traditional chemical methods and is a promising method for the mass production of graphene . To date, electrochemical exfoliation of graphite has been performed mainly in two diﬀerent types of electrolytes, i.e., ionic liquids [12,14] and typical inorganic electrolytes, such as acids and their salts: HCl (e.g., NaCl, KCl), HF (e.g., NaF, KF), H2SO4 (e.g., Na2SO4,K2SO4, (NH4)2SO4,), HNO3 (e.g., NaNO3, KNO3, NH4NO3), H3PO4, NaClO4 [15–24]. Electro-exfoliation in non-electrolytes like H2O2 was likewise performed. The intercalation process, as well as gas evolution, may open up graphene sheets, causing their expansion and exfoliation of the graphene layers . Exfoliation in acidic electrolytes yields graphene ﬂakes of better quality and larger lateral size, but it is impossible to avoid a signiﬁcant amount of oxygen-containing functional groups due to graphite being oxidized by the products of acid electrolysis [10,11,26]. On the other hand, exfoliation in ionic liquids results in a low yield of graphene with has a small lateral size and often functionalization with ionic liquids, disrupting the electronic properties of graphene [14,27]. Therefore, a proper electrolyte system should allow a proper balance between the high purity and high yield of these exfoliated graphene ﬂakes. The studies performed on graphene electro-exfoliation thus far have almost exclusively been focused on the graphene ﬂake splitting itself and the chemical alterations of the ﬂakes due to certain electrode reactions. The same studies overlooked the problem of graphene ﬂakes’ secondary adhesion once the dispersing liquid phase (mainly water) was removed. This causes the electro-exfoliation to be a reversible phenomenon, making the outcome beneﬁts (the presence of separate graphene ﬂakes) hardly applicable in practice. No ﬁxation method of split graphene ﬂakes has been proposed so far. In the recent study we have successfully elaborated a 3D structuring method for durable ﬁxation of graphene ﬂakes obtained from a commercial graphite by wet-chemistry exfoliation . In situ precipitated Na2CO3 nanocrystals or CaCO3 nano-powder were used as a hard template. Graphene ﬂakes were obtained by a wet chemistry exfoliation of commercial graphite. The ﬂakes were premixed with a non-speciﬁc binder and the hard template and then carbonized at temperatures of 700 to 800 ◦C under the ﬂow of nitrogen. The addition of a template allowed the surface area to increase up to 2 1 2 1 287 m g− for the Na2CO3 template and 333 m g− in the case of CaCO3, while the surface area of few 2 1 m g− was noted for the raw graphite. The wet-chemistry method led to an eﬃcient deglomeration of graphene ﬂakes to double-layered (DLG) and few-layered (FLG) graphene. Thus, durably ﬁxed graphene ﬂakes can form 3D graphene sponges. These sponges in turn can substitute typical porous carbon-based materials, e.g., activated carbons, in numerous applications exploiting enhanced speciﬁc surface area and porosity (gas/liquid phase adsorption, electrode processes, etc.). In this work, we demonstrate a highly eﬀective electrochemical exfoliation method in aqueous inorganic salt sodium sulfonate (Na2SO4). We present the ﬁrst case of graphene stabilized with a small amount of carbon obtained from poly(furfuryl alcohol). The graphene ﬂakes which stabilize in a 3D structure were acquired by electroexfoliating two diﬀerent graphite precursors: graphite foil and commercial graphite powder. Additionally, we assumed that split ﬂakes can be durably separated from one another by nanoparticles (Na2CO3, CaCO3) which can be later removed to release nano-voids, i.e., pores. The inﬂuence of process parameters on the characteristics of produced graphene sponges was investigated. Nanomaterials 2019, 9, 971 3 of 12
2. Materials and Methods
2.1. Materials Extra pure graphite was purchased from Merc. The graphene ﬁlms/foils 240 µm thick were provided by Sigma Aldrich. Other reagents i.e., Na2SO4, CaCO3, furfuryl alcohol (FA), HCl and H3PO4 were of analytical purity grade and were obtained from Sigma Aldrich (Warsaw, branch in Poland), POCH (Gliwice, Poland) and SS Nano (Houston, TX, USA).
2.2. Electrochemical Exfoliation Electrochemical exfoliation of extra-pure graphite (Merc) was performed ﬁrst. Such an electro- exfoliation of a powder creates serious experimental obstacles, since the graphite powder is a loose material with no speciﬁc durable shape which could aid holding the mechanical electrode. Therefore, a special electrochemical experimental setup was developed in which the loose powder was electrically charged by temporary contact with a positively charged bottom electrode (platinum plate), as the particles were pulled downwards to the metal surface (sedimentation) by the force of gravity, as depicted in Figure1a. The bottom electrode may be called a working electrode since it was in permanent contact with the graphite powder exposed to electro-exfoliation. A potential of +10 V was set on the electrode, which then played the role of an anode (expected oxidation of anions being present in the electrolyte). After pouring the electrolyte solution (water Na2SO4 1 M solution), graphite powder was sunk and covered by a porous polymeric membrane/separator to avoid graphite/graphene powder spreading throughout the entire electrolyte volume. The electric circuit was completed by placing a movable polymeric plug containing the second platinum electrode (a mesh), on which ground potential was set (0 V) to enable its cathodic function. The movable plug/electrode provided an additional compressing force which, beside natural sedimentation, caused the graphite particles to be in electric contact with the anode, assuming the whole experimental setup is vertically oriented. The meshed structure of the upper electrode (cathode) was permeable for gases evolved during electro-exfoliation. The electro-exfoliation was performed for an experimentally-veriﬁed length of time. After this time passed, the electro-exfoliation was opened and the suspension (water, electrolyte residues, exfoliated graphene ﬂakes, graphite residues) was poured into a beaker and subjected to other chemical manipulations. Additional force/weight may generally be placed on the movable plug, though it was not in the current study. In the second step, we performed the electro-exfoliation of graphite foil (Sigma Aldrich) ca. 3.5 cm ca. 3.5 cm in size. The foil, since it had a ﬁxed shape, served as an anode once the potential of +10 V × was set on it. Thus, the graphite itself played the role of anode while a platinum plate worked as the cathode (after having the ground potential set on it). Anode and cathode zones were not separated by a membrane in this case (Figure1b). The same electrolyte was applied. Electric current passed through the system for an experimentally-veriﬁed period, after that both electrodes (platinum and graphite foil residues) were removed and the suspension (water, electrolyte residues, exfoliated graphene ﬂakes, graphite residues) was poured into a beaker and subjected to other chemical manipulations. Spectacular exfoliation of the foil was observed after only a few minutes, i.e., loose black ﬂakes split from the foil, forming a dark suspension while the foil electrode itself vanished gradually. A direct current (DC) voltage (R&S®HMP2020 power supply) was applied between the platinum and graphite electrodes, and the electrolysis procedure lasted 2 h for graphite powder and 30 min for graphite foil at room temperature. During this process, substances expected to work as a separator of newly exfoliated graphene ﬂakes (denoted later as templates) were added in one of two forms: a nano-powder of CaCO3 (5–40 nm diameter) or a saturated solution of Na2CO3. Nanomaterials 2019, 9, 971 4 of 12 Nanomaterials 2019, 9, x FOR PEER REVIEW 4 of 12
FigureFigure 1. 1. ExperimentalExperimental setup setup of of electroche electrochemicalmical exfoliation exfoliation technique technique for: for: (a) (a graphite) graphite powder, powder, where: where: (1)(1) platinum platinum electrode electrode (cathode), (cathode), (2) (2) platinum platinum el electrodeectrode (anode), (anode), (3) (3) space space for for the the electrolyte electrolyte and and graphitegraphite for for exfoliation, exfoliation, image image of of initial initial graphite graphite powder powder and and the the final ﬁnal graphene graphene after after electrochemical electrochemical exfoliationexfoliation (EG_P); (EG_P); (b) (b) graphite graphite foil, foil, where: where: (1) (1) platinum platinum electr electrodeode (anode), (anode), (2) (2) graphite graphite foil foil (cathode), (cathode), (3)(3) electrolyte, electrolyte, image image of of initial initial graphite graphite foil foil and and the the final ﬁnal graphene graphene after after electrochemical electrochemical exfoliation exfoliation (EG_F).(EG_F).
AGraphene direct current ﬂakes (DC) obtained voltage through (R&S® electrochemicalHMP2020 power graphite supply) splitwas applied were durably between separated the platinum by the anduse graphite of an additional electrodes, agent, and the i.e., electrolysis a template procedure (nano-grains lasted of 2 Na h 2forCO graphite3 or CaCO powder3). Furfuryl and 30 min alcohol for graphitewas added foil alongat room with temperature. H3PO4 (polycondensation During this process, catalyst) substances as a potential expected gluing to work agent. as a Theseparator resulting of newlygraphene–furfuryl exfoliated graphene alcohol (FA)-templateflakes (denoted mass later was as templates) subjected to were heat added treatment in one topolymerize of two forms: PA toa nano-powderpoly(furfuryl of alcohol CaCO (PFA)3 (5–40 (1 nm h atdiameter) 100 ◦C), or then a saturated carbonized solution in a N of2 atmosphere Na2CO3. with a heating rate 1 of 10Graphene◦C min− flakesup to obtained 600 ◦C. through This temperature electrochemica wasl maintained graphite split for were 1 h. durably The process separated was carriedby the useout of in an a tubular additional furnace agent, (Thermolyne i.e., a template F21100). (nano-grains After carbonization, of Na2CO3 or the CaCO samples3). Furfuryl were treated alcohol with was a addedconcentrated along (34%–37%)with H3PO HCl4 (polycondensation solution for 20 min catalyst) (12 mL ofas acida potential was used gluing per 1 gagent. of carbon) The toresulting remove graphene–furfurylCaCO3 and Na2CO alcohol3. They (FA)-template were then washed mass with was distilled subjected water to heat on atreatment Büchner funnelto polymerize until the PA pH to of poly(furfurylthe solution reached alcohol 6–7.(PFA) It was(1 h at dried 100 again°C), then in an carbonized electric furnace in a N at2 atmosphere 100 ◦C for 24 with h. Further a heating in therate text, of 10EG_F_2 °C min and−1 up EG_F_1 to 600 °C. are This used temperature as the denotation was maintained of samples for obtained 1 h. The from process graphite was foilcarried with out CaCO in a3 tubularand Na 2furnaceCO3, respectively. (Thermolyne The F21100). EG_P_2 andAfter EG_P_1 carbonization, samples werethe obtainedsamples fromwere graphitetreated powder,with a concentratedusing CaCO3 (34%–37%)and Na2CO HCl3, respectively. solution for 20 min (12 mL of acid was used per 1 g of carbon) to remove CaCO3 and Na2CO3. They were then washed with distilled water on a Büchner funnel until the pH of the2.3. solution Material reached Characterization 6–7. It was dried again in an electric furnace at 100 °C for 24 h. Further in the text, EG_F_2Structural and parameters EG_F_1 are like used the speciﬁcas the denotation surface area of (Brunauer–Emmett–Teller samples obtained from graphite surface area,foil with SBET ) CaCOand pore3 and structure Na2CO of3, respectively. graphite samples The wereEG_P_2 examined and EG_P_1 using thesamples low-temperature were obtained nitrogen from adsorption graphite powder, using CaCO3 and Na2CO3, respectively.
2.3. Material Characterization
Nanomaterials 2019, 9, 971 5 of 12 method. The relevant isotherms of all samples were measured at 196 C using an automatic adsorption − ◦ instrument, ASAP 2010 (Micromeritics, Norcross, GA, USA). Prior to gas adsorption measurements, the carbon materials were outgassed in a vacuum at 200 ◦C for 2 h. The pore size distribution was derived from adsorption branches by the nonlocalized density functional theory (NLDFT) method. The elemental composition (carbon, nitrogen, and hydrogen) of the materials was analyzed by means of a combustion elemental analyzer (Vario MACRO CHN, Elementar Analysensysteme GmbH). The morphology of the samples was analyzed using scanning electron microscopy (SEM, 1430 VP, LEO Electron Microscopy Ltd., Cambridge, UK) and high-resolution transmission electron microscopy (HRTEM, FEI Europe production, model Tecnai F20 X-Twin). The samples were examined using Raman spectroscopy–microscope: Renishaw InVia (Renishaw plc, Gloucestershire, UK), laser: Modu-Laser Stellar-REN, Multi-Line (maximum Power 150 mW), camera: Leica DM1300M Inﬁnity 1, lens: Leica, N PLAN L50 /0.5. All spectra were collected at ambient temperatures with a 532 nm excitation × wavelength. Atomic force microscopy (AFM) investigations were measured by Scanning Probe Microscope (SPM) produced by Veeco (Digital Instrument, Plainview, NY, USA).
3. Results and Discussion Graphene ﬂakes can be produced from graphite, either in the form of a foil or a powder electrode, by exfoliation in 1 M Na2SO4 solution, wherein the same electric charges placed on the graphite domains create repulsive forces. Additionally, when a positive potential is set on the working electrode 2 (either graphite foil or graphite powder), anions (mainly SO4 −) absorb on active sites of the graphite electrodes and oxidize to gaseous oxygen. The anions and evolved gas may penetrate into the interstitial space between graphene layers (in powder or foil) and expand the materials to the point of splitting them into less agglomerated forms, like single-layered graphene (SLG) and few-layered graphene (FLG). Gas (mainly oxygen) evolution accelerates the switching rate of graphite to graphene. We propose a mechanism of electrochemical exfoliation using an additional substrate of Na3CO3 (Figure2a) or CaCO 3 (Figure2b). In the former procedure (Figure2a), to a 1 M Na 2SO4 electrolyte solution a small volume of N-methyl-2-pyrrolidone (NMP) and cetyltrimethylammonium chloride solution (CTAC) was added. After electrochemical exfoliation, the resulting product was ultrasonicated for 30 min, then a Na2CO3 solution at a concentration of about 16.9% was added; the mixture was left on a magnetic stirrer for 1 h, then sonicated again for 1h. The samples were then washed with distilled water on a Büchner funnel. To evaporate the distilled water, the mass was dried in an electric oven at 80 ◦C for 24 h. In the second method (Figure2b), instead of Na 2CO3, CaCO3 nanoparticles with a size range of 5–40 nm were added. Raman spectroscopy is a method particularly useful for characterizing graphene/graphite type materials [29,30]. Among others, Raman spectroscopy makes it possible to distinguish graphite-based materials from graphene-based ones, to estimate graphene layers stacked together (SLG – Single Layered Graphene, FLG – Few Layered Graphene, and MLG – Multi Layered Graphene diﬀerentiation), and to resolve other problems. Figure3a–d provides Raman spectra of graphene obtained in the two ways with two diﬀerent separators, Na2CO3 and CaCO3. Additionally, Table1 presents the position and intensity of the peaks in Figure3. Figure3b,d show the Raman spectra of the graphene products obtained with diﬀerent separators, where the increased value of ID/IG suggests the decrease of graphene agglomerate thickness. As shown in Table1, a strong relative intensity of the 2D peak indicates fewer stacked layers, which in foil exfoliation with CaCO3 is beneﬁcial for the formation of graphene. The presence of graphitic carbon in the EG_F_2 and EG_F_1 samples (Figure3b) revealed 1 the well-documented D and G bands at 1351 and 1579 cm− , with an ID/IG ratio of 0.53 and 0.13, respectively. An analysis of the Raman spectra for pristine graphite foil (Figure3a) and pristine graphite powder (Figure3c) leads us to believe that the foil is closer to an ideal graphene material than the powder. This conclusion results from the ID/IG ratio, which is only 0.17 for the foil and 0.59 for the powder. Furthermore, the conclusion is supported by the observed shape of the D band, which is very broad in the powder spectrum. Nanomaterials 2019, 9, 971 6 of 12 Nanomaterials 2019, 9, x FOR PEER REVIEW 6 of 12
FigureFigure 2.2. SchematicSchematic illustration illustration of of the the mechanism mechanism of ofelectrochemical electrochemical cathodic cathodic exfoliation exfoliation with: with: (a) Na2CO3 and (b) CaCO3 as a separator and poly(furfuryl alcohol) (PFA) as a stabilizer. (a) Na2CO3 and (b) CaCO3 as a separator and poly(furfuryl alcohol) (PFA) as a stabilizer.
TableRaman 1. Raman spectroscopy peak positions is a method and intensities particularly for the productsuseful for obtained characterizing from samples graphene/graphite in diﬀerent series. type materials [29,30]. Among others, Raman spectroscopy makes it possible to distinguish graphite-based D peak G peak 2D peak materials fromSample graphene-based ones, to estimate graphene layers stacked togetherID/IG (SLGI2D/I G– Single 1 I 1 I 1 I Layered Graphene, FLG(cm –− Few) Layered(cm −Graphene,) and(cm −MLG) – Multi Layered Graphene differentiation),Graphite and foil to resolve 1349.3 other 694 problems. 1582.3 Figure 4158 3a–d 2718.0 provides 2343 Raman 0.17 spectra of 0.56 graphene Graphite powder 1343.4 1781 1578.0 2994 2705.6 1138 0.59 0.38 obtained in the two ways with two different separators, Na2CO3 and CaCO3. Additionally, Table 1 EG_P_2 1334.7 2868 1592.2 4081 2867.5 1207 0.70 0.30 presents theEG_P_1 position and 1330.1intensity 2764of the peaks 1587.6 in Figure 3822 3. 2868.7Figure 3b,d 1066 show 0.72the Raman 0.28 spectra of the grapheneEG_F_2 products obtained 1339.1 with 6058 different 1578.0 separators,11,534 where2705.6 the increased 4211 value 0.53 of ID 0.37/IG suggests the decreaseEG_F_1 of graphene 1346.2agglomerate 1343 thickness. 1568.9 As10,186 shown 2692.1in Table 1, 3888 a strong 0.13 relative 0.38intensity of the 2D peak indicates fewer stacked layers, which in foil exfoliation with CaCO3 is beneficial for the formation of graphene. The presence of graphitic carbon in the EG_F_2 and EG_F_1 samples (Figure 3b) revealed the well-documented D and G bands at 1351 and 1579 cm−1, with an ID/IG ratio of 0.53 and 0.13, respectively. An analysis of the Raman spectra for pristine graphite foil (Figure 3a) and pristine graphite powder (Figure 3c) leads us to believe that the foil is closer to an ideal graphene material than the powder. This conclusion results from the ID/IG ratio, which is only 0.17 for the foil
Nanomaterials 2019, 9, x FOR PEER REVIEW 7 of 12
and 0.59 for the powder. Furthermore, the conclusion is supported by the observed shape of the D band, which is very broad in the powder spectrum.
Table 1. Raman peak positions and intensities for the products obtained from samples in different series.
D peak G peak 2D peak Sample ID/IG I2D/IG (cm−1) I (cm−1) I (cm−1) I Graphite foil 1349.3 694 1582.3 4158 2718.0 2343 0.17 0.56 Graphite powder 1343.4 1781 1578.0 2994 2705.6 1138 0.59 0.38 EG_P_2 1334.7 2868 1592.2 4081 2867.5 1207 0.70 0.30 EG_P_1 1330.1 2764 1587.6 3822 2868.7 1066 0.72 0.28 EG_F_2 1339.1 6058 1578.0 11,534 2705.6 4211 0.53 0.37 Nanomaterials 2019, 9, 971 7 of 12 EG_F_1 1346.2 1343 1568.9 10,186 2692.1 3888 0.13 0.38
FigureFigure 3. 3.Raman Raman spectra spectra of of ( a(a)) graphite graphite foil, foil, ( b(b)) EG_F_2 EG_F_2 and and EG_F_1, EG_F_1, ( c(c)) graphite graphite powder, powder, (d (d)) EG_P_2 EG_P_2 andand EG_P_1 EG_P_1 samples. samples. Pore Pore size size distribution distribution curves curves of grapheneof graphene samples samples obtained obtained from from graphite graphite (e) foil (e) andfoil ( fand) powder. (f) powder.
ToTo conﬁrm confirm the the presence presence of double-to-few-layered of double-to-few-layered stabilized stabilized graphene, graphene, SEM and SEM HRTEM and analysisHRTEM wasanalysis used. was A SEM used. image A SEM of PFA-graphene image of PFA-graphene is shown in is Figure shown4. in SEM Figure studies 4. SEM the fracturestudies the surface fracture in puresurface graphene in pure/carbon graphene/carbon from PFA (Figure from4). PFA Prior (Figure work has 4). shown Prior thatwork graphene has shown aggregates that graphene can be seenaggregates in SEM, can but be it seen is quite in SEM, diﬃcult but toit is image quite individual difficult to dispersion image individual graphene dispersion sheets in graphene composites sheets at lowin composites weight fractions. at low We weight observed fractions. no signs We of observ aggregation.ed no signs We could of aggregation. not observe We individual could not graphene observe sheetsindividual in the graphene fracture surface sheets ofin graphene.the fracture surface of graphene. The HRTEM technique allowed the dispersion of graphene sheets and was stabilized with small amount of carbon from PFA. Thin-layer graphene sheets were produced at a high yield with large ﬂake sizes (Figure5). Few-layered graphene sheets can be seen in Figure5. Images of the sheet edges are visible in Figures5b and6d; those in Figure5d indicate that the sheets are 2–4 or more layers thick. The HRTEM images allow to evaluate the size of electrochemically exfoliated graphene sheets as 0.7 4 − µm. Nanomaterials 2019, 9, x FOR PEER REVIEW 8 of 12
Nanomaterials 2019, 9, 971 8 of 12 Nanomaterials 2019, 9, x FOR PEER REVIEW 8 of 12
Figure 4. SEM images of (a, b) EG_F_2 and (c, d) EG_F_1.
The HRTEM technique allowed the dispersion of graphene sheets and was stabilized with small amount of carbon from PFA. Thin-layer graphene sheets were produced at a high yield with large flake sizes (Figure 5). Few-layered graphene sheets can be seen in Figure 5. Images of the sheet edges are visible in Figures 5b,6d; those in Figure 5d indicate that the sheets are 2–4 or more layers thick.
The HRTEM images allow to evaluate the size of electrochemically exfoliated graphene sheets as 0.7−4 μm. FigureFigure 4. 4.SEM SEM images images of of (a ,(a,b) b) EG_F_2 EG_F_2 and and (c, d(c,) EG_F_1.d) EG_F_1.
The HRTEM technique allowed the dispersion of graphene sheets and was stabilized with small amount of carbon from PFA. Thin-layer graphene sheets were produced at a high yield with large flake sizes (Figure 5). Few-layered graphene sheets can be seen in Figure 5. Images of the sheet edges are visible in Figures 5b,6d; those in Figure 5d indicate that the sheets are 2–4 or more layers thick. The HRTEM images allow to evaluate the size of electrochemically exfoliated graphene sheets as 0.7−4 μm.
FigureFigure 5. High-resolution 5. High-resolution transmission transmission electron electron microscopy microscopy (HRTEM) (HRTEM) images images of (a–c )of EG_F_2 (a–c) EG_F_2 and and (d–f) EG_F_1.(d–f) EG_F_1.
In orderIn order to get to information get information on the on thickness the thickness and lateral and lateral size of size electrochemically of electrochemically exfoliated exfoliated graphenegraphene sheets, sheets, AFM analysisAFM analysis was performed was performed using using EG_P_2 EG_P_2 and EG_F_2 and EG_F_2 samples samples subjected subjected to to sonication in ethanol. The results are presented in Figure6. Typical graphene sheet thickness is about
2 nm.Assuming that the thickness of single layered graphene is 0.51 nm  and the interlayer distance is 0.34 nmFigure the 5. measured High-resolution value transmission corresponds electron to three microscopy layered graphene: (HRTEM) 3images0.51 of nm (a–c)+ 2EG_F_20.34 and nm = × × 2.17 nm.(d–f) This EG_F_1. result is consistent with Raman spectroscopy studies which also suggest the performed electro-exfoliation delivers few-layered graphene mainly. In order to get information on the thickness and lateral size of electrochemically exfoliated graphene sheets, AFM analysis was performed using EG_P_2 and EG_F_2 samples subjected to
Nanomaterials 2019, 9, x FOR PEER REVIEW 9 of 12
sonication in ethanol. The results are presented in Figure 6. Typical graphene sheet thickness is about 2 nm. Assuming that the thickness of single layered graphene is 0.51 nm  and the interlayer distance is 0.34 nm the measured value corresponds to three layered graphene: 3 × 0.51 nm + 2 × 0.34 nm = 2.17 nm. This result is consistent with Raman spectroscopy studies which also suggest the Nanomaterials 2019, 9, 971 9 of 12 performed electro-exfoliation delivers few-layered graphene mainly.
FigureFigure 6. Atomic6. Atomic force force microscopy microscopy (AFM) (AFM) analysis analysis together together with with height height proﬁleprofile ofof ((aa)) EG_P_2,EG_P_2, (b) (b) EG_F_2.EG_F_2.
Generally,Generally, other other communications communications on exfoliation on exfoliation provide provide no analysis no analysis of structural of structural parameters parameters such as speciﬁcsuch as surface specific area surface and area pore and structure. pore structure. This problem This problem may be regardedmay be regard as a kinded as of a blankkind of spot blank whichspot is yetwhich tobe is ﬁlled.yet to Webe assumefilled. We that assume thesestructural that these parameters structural areparameters diﬃcult toare measure difficult when to measure the exfoliatedwhen the graphene exfoliated ﬂakes graphene are not flakes secured are against not secured secondary against stacking secondary (due stacking to inter-ﬂake (due attractiveto inter-flake forcesattractive known asforces spontaneous known as pi–pi spontaneous stacking). pi–pi The currentstacking). study The is current based onstudy the separationis based on (addition the separation of nano-templates)(addition of nano-templates) and ﬁxation (carbon and fixation bridges (carbon originating bridges from originating PFA) of exfoliated from PFA) ﬂakes. of exfoliated Thus, in theflakes. caseThus, of these in the samples, case of i.e., these graphene samples, sponges, i.e., graphene structural sp parametersonges, structural like surface parameters area and like pore surface structure area and becomepore measurable.structure become Our study measurable. is unique Our among study reports is unique dealing among with reports this problem. dealing with this problem. The results regarding speciﬁc surface area (S ) are given in Table2 for the two di ﬀerent The results regarding specific surface areaBET (SBET) are given in Table 2 for the two different graphene-ﬂake separators, i.e., Na CO or CaCO . The highest S was found for samples obtained graphene-flake separators, i.e.,2 Na23CO3 or CaCO3 3. The highestBET SBET was found for samples obtained with CaCO as a separator. Both electro-exfoliation approaches (graphene foil and powder) yielded with CaCO3 3 as a separator. Both electro-exfoliation approaches (graphene foil and powder) yielded samples with the highest values of S , i.e., EG_F_2 with 121 m2 g 1 and EG_P_2 with 220 m2 g 1. These samples with the highest valuesBET of SBET, i.e., EG_F_2 with −121 m2 g−1 and EG_P_2 with− 220 m2 g−1. valuesThese were values calculated were calculated using the regressionusing the regression of data from of thedata original from the nitrogen original adsorption nitrogen adsorption at –196 ◦C. at – The196 same °C. data The letsame us estimatedata let us pore estimate size distribution pore size di bystribution using the by widely using acceptedthe widely nonlocal-density accepted nonlocal- functionaldensity theory functional (NLDFT) theory model (NLDFT) [32–34 model]. Figure [32–34].3e,f show Figu porere 3e,f size show distribution pore size (PSD) distribution of the EG_F_2, (PSD) of EG_F_1the EG_F_2, and EG_P_2, EG_F_1 EG_P_1 and EG_P_2, samples. EG_P_1 Interestingly, samples. allInterestingly, the PSD curves all the only PSD cover curves the only range cover of the micropores.range of Themicropores. PSD function The PSD for foil-originatedfunction for foil-originated samples is unique samples because is unique of two because overlapping of two peaksoverlapping in which maximapeaks in occurwhich at maxima 9.3, 11.7 occur (Figure at 9.3,3e). 11 One.7 (Figure may consider 3e). One the may distribution consider the as distribution almost monomodal,as almost which monomodal, is in contrast which to is the in bimodal contrast PSD to the function bimodal recorded PSD forfunction graphene recorded sponges for created graphene by thesponges electro-exfoliation created by the of electro-exfoliation graphene powder. of For grap twohene graphene powder. samples For two obtained graphene from samples graphite obtained foil we canfrom observe graphite main foil peakswe can at observe 0.9, 1.2, main and 1.7peaks nm at (Figure 0.9, 1.2,3e). and PSD 1.7 curves nm (Figure (Figure 3e).3f) PSD show curves that the (Figure dominant3f) show pore that sizes the were dominant similar pore for both sizes samples were simi of graphenelar for both obtained samples from of graphite graphene powder obtained at 0.8, from 1.8 nmgraphite and 0.9, powder 1.7 nm at of 0.8, EG_P_2 1.8 nm and and EG_P_1, 0.9, 1.7 nm respectively. of EG_P_2 and EG_P_1, respectively. The chemical composition was investigated using CHN combustion elemental analysis and the Table 2. Speciﬁc surface area (S ) and elemental content of carbon, hydrogen, and nitrogen. results are presented in Table 2.BET Generally, the carbon content was very high and typical for real graphene-based materials , i.e., it is proven that totalContent carbon (wt%) content ranges from 90.0wt% to 2 1 Sample SBET (m g ) 94.3wt%. Combustion elemental analysis− also C%H%N%delivers information on the content of oxygen. Assuming that the content of unidentified elements (complement to 100% for each sample) is the EG_F_2 121 93.0 0.6 0.2 content of oxygen,EG_F_1 the carbon-to-oxygen 52 ratio (C/O 94.3 ratio) examined 0.3 by 0.1elemental analysis is high (from 11.2 to 17.8)EG_P_2 and typical to 220graphene not 90.0to graphene1.8 oxide [15,22]. 0.2 Therefore, the obtained sponges can be consideredEG_P_1 to consist 103 of graphene 90.5 flakes. The 2.0C/O ratio is 0.2considerably higher for the foil-originated samples, which is in accordance with the Raman spectroscopy results, proving that The chemical composition was investigated using CHN combustion elemental analysis and the results are presented in Table2. Generally, the carbon content was very high and typical for real graphene-based materials , i.e., it is proven that total carbon content ranges from 90.0wt% to 94.3wt%. Combustion elemental analysis also delivers information on the content of oxygen. Assuming Nanomaterials 2019, 9, 971 10 of 12 that the content of unidentiﬁed elements (complement to 100% for each sample) is the content of oxygen, the carbon-to-oxygen ratio (C/O ratio) examined by elemental analysis is high (from 11.2 to 17.8) and typical to graphene not to graphene oxide [15,22]. Therefore, the obtained sponges can be considered to consist of graphene ﬂakes. The C/O ratio is considerably higher for the foil-originated samples, which is in accordance with the Raman spectroscopy results, proving that the foil likely consists of graphene domains. Some XPS (X-Ray Photoemission Spectroscopy) studies as well as SEM-EDX studies (Scanning Electron Microscopy combined with Energy Dispersive X-Ray module) did not reveal the content of heavier elements (like Ca, Na, P, etc.) is higher than 1%. Thus, our assumption that unidentiﬁed element content (Table2) may be ascribed to oxygen is justiﬁed and realistic.
4. Conclusions In conclusion, an accessible method was developed and demonstrated for obtaining few-layered graphene directly from graphite by electro-exfoliation and 3D stabilization by means of carbonized PFA as a stabilizer and certain inorganic carbonates as templates. The obtained samples can be treated as porous carbon sponges built of graphene ﬂakes. The study indicates that the presence of carbonized PFA is critical for stabilizing the graphene and improving the surface parameters; the speciﬁc surface area increased several times compared to the starting material (graphite). The relatively high graphene purities and excellent stabilization with PFA show both methods to be promising ways of developing porous graphene. The morphological properties include the nanostructure of graphene powder with diﬀerent sizes, characterized by SEM and HRTEM. The structural properties indicate a high quality for graphene, as determined by Raman spectroscopy. Low-cost and environmentally friendly production of such high-quality graphene is important, not only for future-generation electronics, but also for large-scale applications, such as composite materials, supercapacitors, fuel-cells, and batteries. Any practical application requires upscaling of the electrochemical arrangement and a cost calculation. The economic aspect of electrochemical exfoliation directly points to powdered graphite of high purity since its market prices are deﬁnitely much lower than the price of graphene foil. Experimental setup for exfoliation of graphite powder which was tested in the current project can be enlarged as single cell, but also small volume single cells may be used as a cell array. The presented electro-exfoliation approach has one general advantage over typical wet chemistry approaches: the inevitable chemical reagents i.e., electrolytes are common, inexpensive, and relatively easy to utilize. An upscale of the electrochemical cell will be the target of subsequent studies.
Author Contributions: Conceptualization J.P.L; methodology J.P.L. and A.I.; formal analysis A.I. and M.S.; investigation A.I., M.S., and P.K.; writing—original draft preparation J.P.L. and A.I.; review and editing A.I. and J.P.L.; visualization A.I. and M.S.; supervision J.P.L; project administration J.P.L. and A.I.; funding acquisition J.P.L. Funding: This work was supported by the National Science Centre (Poland) grant 2016/23/B/ST5/00658. Acknowledgments: All experimental work (synthesis, analysis) was supported by the National Science Centre (Poland) grant 2016/23/B/ST5/00658. Conﬂicts of Interest: The authors declare no conﬂict of interest.
1. Dixit, A.; Dixit, D.; Chandrodaya, V.V.; Kajla, A. Graphene: A new era of technology. Int. J. Emerg. Technol. Adv. Eng. 2013, 3, 4–7. 2. Neto, A.C.; Guinea, F.; Peres, N.M.; Novoselov, K.S.; Geim, A.K. The electronic properties of graphene. Rev. Mod. Phys. 2009, 81, 109. [CrossRef] 3. Park, S.; Ruoﬀ, R.S. Chemical methods for the production of graphenes. Nature Nanotechnol. 2009, 4, 217. [CrossRef][PubMed] 4. Nuvoli, D.; Alzari, V.; Sanna, R.; Scognamillo, S.; Piccinini, M.; Peponi, L.; Kenny, J.M.; Mariani, A. The production of concentrated dispersions of few-layer graphene by the direct exfoliation of graphite in organosilanes. Nanoscale Res. Lett. 2012, 7, 674. [CrossRef][PubMed] Nanomaterials 2019, 9, 971 11 of 12
5. Scaﬀaro, R.; Maio, A. Integrated ternary bionanocomposites with superior mechanical performance via the synergistic role of graphene and plasma treated carbon nanotubes. Compos. Part. B: Eng. 2019, 168, 550–559. [CrossRef] 6. Scaﬀaro, R.; Maio, A.; Lo Re, G.; Parisi, A.; Busacca, A. Advanced piezoresistive sensor achieved by amphiphilic nanointerfaces of graphene oxide and biodegradable polymer blends. Compos. Sci. Technol. 2018, 156, 166–176. [CrossRef] 7. Scaﬀaro, R.; Maio, A. A green method to prepare nanosilica modiﬁed graphene oxide to inhibit nanoparticles re-aggregation during melt processing. Chem. Eng. J. 2017, 308, 1034–1047. [CrossRef] 8. Bonaccorso, F.; Lombardo, A.; Hasan, T.; Sun, Z.; Colombo, L.; Ferrari, A.C. Production and processing of graphene and 2d crystals. Mater. Today 2012, 15, 564–589. [CrossRef] 9. Tripathi, P.; Patel, C.; Prakash, R.; Shaz, M.; Srivastava, O. Synthesis of high-quality graphene through electrochemical exfoliation of graphite in alkaline electrolyte. arXiv preprint 2013, arXiv:1310.7371. 10. Su, C.-Y.; Lu, A.-Y.; Xu, Y.; Chen, F.-R.; Khlobystov, A.N.; Li, L.-J. High-quality thin graphene ﬁlms from fast electrochemical exfoliation. ACS Nano 2011, 5, 2332–2339. [CrossRef] 11. Parvez, K.; Li, R.; Puniredd, S.R.; Hernandez, Y.; Hinkel, F.; Wang, S.; Feng, X.; Müllen, K. Electrochemically Exfoliated Graphene as Solution-Processable, Highly Conductive Electrodes for Organic Electronics. ACS Nano 2013, 7, 3598–3606. [CrossRef][PubMed] 12. Lu, J.; Yang, J.-x.; Wang, J.; Lim, A.; Wang, S.; Loh, K.P. One-Pot Synthesis of Fluorescent Carbon Nanoribbons, Nanoparticles, and Graphene by the Exfoliation of Graphite in Ionic Liquids. ACS Nano 2009, 3, 2367–2375. [CrossRef][PubMed] 13. Zhong, Y.L.; Tian, Z.; Simon, G.P.; Li, D. Scalable production of graphene via wet chemistry: Progress and challenges. Mater. Today 2015, 18, 73–78. [CrossRef] 14. Liu, N.; Luo, F.; Wu, H.; Liu, Y.; Zhang, C.; Chen, J. One-Step Ionic-Liquid-Assisted Electrochemical Synthesis of Ionic-Liquid-Functionalized Graphene Sheets Directly from Graphite. Adv. Funct. Mater. 2008, 18, 1518–1525. [CrossRef] 15. Parvez, K.; Wu, Z.-S.; Li, R.; Liu, X.; Graf, R.; Feng, X.; Müllen, K. Exfoliation of graphite into graphene in aqueous solutions of inorganic salts. J. Am. Chem. Soc. 2014, 136, 6083–6091. [CrossRef][PubMed] 16. Chen, C.-H.; Yang, S.-W.; Chuang, M.-C.; Woon, W.-Y.; Su, C.-Y. Towards the continuous production of high crystallinity graphene via electrochemical exfoliation with molecular in situ encapsulation. Nanoscale 2015, 7, 15362–15373. [CrossRef][PubMed] 17. Rao, K.S.; Senthilnathan, J.; Liu, Y.-F.; Yoshimura, M. Role of peroxide ions in formation of graphene nanosheets by electrochemical exfoliation of graphite. Sci. Rep. 2014, 4, 4237. [CrossRef][PubMed] 18. Hossain, S.T.; Wang, R. Electrochemical exfoliation of graphite: Eﬀect of temperature and hydrogen peroxide addition. Electrochimica Acta 2016, 216, 253–260. [CrossRef] 19. Zhou, M.; Tang, J.; Cheng, Q.; Xu, G.; Cui, P.; Qin, L.-C. Few-layer graphene obtained by electrochemical exfoliation of graphite cathode. Chem. Phys. Lett. 2013, 572, 61–65. [CrossRef] 20. Jibrael, R.I.; Mohammed, M.K. Production of graphene powder by electrochemical exfoliation of graphite electrodes immersed in aqueous solution. Optik 2016, 127, 6384–6389. [CrossRef] 21. Hamra, A.; Lim, H.; Chee, W.; Huang, N. Electro-exfoliating graphene from graphite for direct fabrication of supercapacitor. Appl. Surf. Sci. 2016, 360, 213–223. [CrossRef] 22. Lee, J.-W.; Kim, M.; Na, W.; Hong, S.M.; Koo, C.M. Fabrication of high quality graphene nanosheets via a spontaneous electrochemical reaction process. Carbon 2015, 91, 527–534. [CrossRef] 23. Xu, J.; Shi, Z.; Zhang, X.; Martin Haarberg, G. Mechanism of graphene formation by graphite electro-exfoliation in ionic liquids-water mixtures. Mater. Res. Express 2014, 1, 045606. [CrossRef] 24. Zeng, Z.; Yin, Z.; Huang, X.; Li, H.; He, Q.; Lu, G.; Boey, F.; Zhang, H. Single-Layer Semiconducting Nanosheets: High-yield preparation and device fabrication. Angew. Chem. Int. Ed. 2011, 50, 11093–11097. [CrossRef][PubMed] 25. Yu, P.; Lowe, S.E.; Simon, G.P.; Zhong, Y.L. Electrochemical exfoliation of graphite and production of functional graphene. Curr. Opin. Colloid Interface Sci. 2015, 20, 329–338. [CrossRef] 26. Liu, J.; Yang, H.; Zhen, S.G.; Poh, C.K.; Chaurasia, A.; Luo, J.; Wu, X.; Yeow, E.K.L.; Sahoo, N.G.; Lin, J.; et al. A green approach to the synthesis of high-quality graphene oxide ﬂakes via electrochemical exfoliation of pencil core. RSC Adv. 2013, 3, 11745–11750. [CrossRef] Nanomaterials 2019, 9, 971 12 of 12
27. Shang, N.G.; Papakonstantinou, P.; Sharma, S.; Lubarsky, G.; Li, M.; McNeill, D.W.; Quinn, A.J.; Zhou, W.; Blackley, R. Controllable selective exfoliation of high-quality graphene nanosheets and nanodots by ionic liquid assisted grinding. Chem. Commun. 2012, 48, 1877–1879. [CrossRef] 28. Kamedulski, P.; Ilnicka, A.; Lukaszewicz, J.P.; Skorupska, M. Highly eﬀective three-dimensional functionalization of graphite to graphene by wet chemical exfoliation methods. Adsorption 2019, 25, 631–638. [CrossRef] 29. Bokobza, L.; Bruneel, J.-L.; Couzi, M. Raman spectra of carbon-based materials (from graphite to carbon black) and of some silicone composites. C 2015, 1, 77–94. [CrossRef] 30. Hodkiewicz, J.; Scientiﬁc, T. Characterizing carbon materials with Raman spectroscopy. Appl. Note 2010, 51946. 31. Ni, Z.; Wang, H.; Kasim, J.; Fan, H.; Yu, T.; Wu, Y.; Feng, Y.; Shen, Z. Graphene thickness determination using reﬂection and contrast spectroscopy. Nano Lett. 2007, 7, 2758–2763. [CrossRef][PubMed] 32. Ravikovitch, P.I.; Neimark, A.V. Characterization of Micro- and Mesoporosity in SBA-15 Materials from Adsorption Data by the NLDFT Method. J. Phys. Chem. B 2001, 105, 6817–6823. [CrossRef] 33. Jagiello, J.; Olivier, J.P. 2D-NLDFT adsorption models for carbon slit-shaped pores with surface energetical heterogeneity and geometrical corrugation. Carbon 2013, 55, 70–80. [CrossRef] 34. Landers, J.; Gor, G.Y.; Neimark, A.V. Density functional theory methods for characterization of porous materials. Colloids Surf. A: Physicochemical Eng. Aspects 2013, 437, 3–32. [CrossRef]
© 2019 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).